COMPARISON OF SHEAR & TENSILE BOND
STRENGTH OF BRACKETS BONDED WITH A
CONVENTIONAL (2 STEP) AND A SELF- ETCH
(ALL IN ONE) BONDING SYSTEMS
-AN IN VITRO STUDY
Dissertation submitted to
THE TAMILNADU Dr. M.G.R. MEDICAL UNIVERSITY
In partial fulfillment for the Degree of
MASTER OF DENTAL SURGERY
DEPARTMENT OF ORTHODONTICS
This is to certify that this dissertation titled “COMPARISON OF
SHEAR & TENSILE BOND STRENGTH OF BRACKETS BONDED
WITH A CONVENTIONAL (2 STEP) AND A SELF- ETCH (ALL IN
ONE) BONDING SYSTEMS -AN IN VITRO STUDY” is a bonafide
research of work done by Dr. B.AKILANANTH. Under my guidance
during his postgraduate study period between 2009-2012.
This dissertation is submitted to THE TAMILNADU DR.M.G.R.
MEDICAL UNIVERSITY, in partial fulfilment for the degree of Master of
Dental Surgery in Branch V-Orthodontics.
It has not been submitted (partially or fully)for the award of any other
degree or diploma.
Dr. R .K. VIJAYAKUMAR, MDS,
Guide, Professor and Head
Department of Orthodontics,
Sri Ramakrishna Dental College and
Dr. V. PRABHAKAR, MDS
Sri Ramakrishna Dental College and Hospital,
This enterprise would not have been possible without Master’s grace and spiritual
guidance. I bow before the Almighty who with his immense bountiful nature showered
blessings on me.
Words are nothing but a medium to express my respect and gratitude to my
respected teacher Dr. R.K.VIJAYAKUMAR, Professor and Head, Department of
Orthodontics and Dentofacial Orthopedics Sri Ramakrishna. Dental College and Hospital,
Coimbatore, for his guidance in completing this dissertation.
Expressions are inadequate to convey my immense gratitude to our Reader
Dr. Jegadeep Raju for his keen interest, moral support and encouragement throughout
I extend my heartfelt thanks to our senior lecturers Dr. S.D. Milling Tania,
Dr. Sam Thomas and Dr. S. Fiyaz Ahmed, Sri Ramakrishna Dental College and
Hospital, Coimbatore for providing me with all the necessary support whenever needed.
I wholeheartedly thank our principal Dr. Prabakar, for giving me permission to
utilize the facilities available in our college for my work.
Iam grateful to Dr. Padmanaban., Professor Emeritus, Dr. Joshi C. Haran and
K. Ramesh kumar, Professors Mechanical Department, Dr. C. Elangovan, Asst.
professor and Mr. Radhakrishnan Teaching Assistant, Amirtha School of Engineering
Ettimadai, Coimbatore for giving me their precious time and allowing me to use the
strength testing machine as per my study requirements.
I also extend my gratidude to my co PG Dr. Aprose Kanna and all my junior
colleagues Dr. Suresh, Dr. Archana, Dr .Pradeep and Dr. Yamuna for their help.
Finally I would like to thank my parents, my wife and children for their
understanding, concern and exceptional love which gave the strength and fitness of mind
to complete this task on time.
I express my apology for not thanking each and every body who was important for
the successful realisation of this thesis.
1. INTRODUCTION 1
2. REVIEW OF LITERATURE 5
3. MATERIALS AND METHODS 26
4. RESULTS 37
5. DISCUSSION 51
6. SUMMARY AND CONCLUSION 62
7. BIBLIOGRAPHY 64
Orthodontic metal bands made of platinum were used in 1870s by W.E.Magill,
(which has been used centuries ago by the Phoenicians, and was later reintroduced by
various men like C.A Harris) were cemented to the teeth by oxychloride of zinc cement
and have been in existence for more than 100 years. The introduction of acid etching
technique by Buonocore in 1955
and the development of orthodontic resins (Diglycidyl
ether of Bisphenol-A, with a polyamide curing agent) by Bowen
, has replaced the
banding with bonding, making a new era in orthodontic history. This offered exciting
possibilities of a more aesthetic appearance for the patient with other advantages of
having no band spaces to close after treatment, less gingival irritation, increased ease of
plaque removal etc.
Ever since the inception of bonding to orthodontics, the materials used for
bonding have undergone considerable improvement from time to time. Present day
adhesives bonding systems claim superior bonding characteristics, even in difficult to
isolate and hard to reach areas. The future of bonding is promising as these material
developments in term of adhesive bond strength, brackets design, and technical details are
continually occurring at a rapid rate.
In 1955 Bunocore laid the foundation for adhesive restoration and preventive
dentistry by introducing etching enamel which renders it more receptive to adhesion and
advocated use of 85% phosphoric acid for 30 seconds. Subsequently, Gwinnett, Matsui
Suggested that formation of resin tag from the adhesive was the primary
mechanism of attachment. Etching removes about 10 micron of enamel and creates
porous layer that ranges from 5 to 10 micron depth.
Silverstone reported that phosphoric acid concentrations between 30% and 40%
provide enamel surface that have the most retentive appearance and as a result of these
studies most of the commercial etchants now available are with 37% concentration.
One of the potential disadvantages of etching with phosphoric acid is that the acid
causes demineralization of the most superficial layer. To control excessive enamel loss,
maleic and polyacrylic acids have been used as alternatives for phosphoric acid. The use
of these acids were found to result in a reduction in bond strength
Conventional resin composites require the use of 3 different agents (enamel
conditioner, primer, and adhesive resin) to bond orthodontic brackets to enamel. Because
of their hydrophobic properties, these products require completely dry and isolated fields
to obtain clinically acceptable bond strength.
However, a variety of clinical conditions do not permit ideal isolation. Moisture
contamination is considered the most common reason for bond failure. When etched
enamel becomes wet, most of the pores become plugged, and resin penetration is
resulting in resin tags of insufficient number and length. Even momentary
saliva contamination adversely affects the bond, because saliva deposits an organic
adhesive coating in the first few seconds of exposure that is resistant to washing. Thus, it
would be advantageous to be able to bond to enamel in a wet environment, particularly in
hard-to-reach areas, such as around second molars or partially erupted and impacted teeth.
To address the problem of contamination, manufacturers introduced hydrophilic
bonding materials that promised successful bonding to a moisture-contaminated enamel
surface. Some hydrophilic enamel primers for orthodontic treatment are formulated with
alcohol or acetone to displace moisture from the isolated enamel surface.Transbond
Moisture Insensitive Primer (MIP; 3M Unitek, Monrovia, Calif) contains a hydrophilic
primer dissolved in acetone and is recommended for use on dry or wet etched enamel
with either self- or light-cured bonding agents.
More recently, newly formulated self-etching primers were developed to combine
conditioning and priming agents into a single acidic primer with simultaneous use on
enamel and dentin, thus eliminating the need for separate etching, rinsing, and drying.
This type of product would have the advantage of a faster and simplified application
technique and allow effective conditioning and priming of enamel and dentin in 1 step,
without sacrificing adequate bond strength.
These self-etch primers help the clinician save time, reduce cross-contamination,
and reduce wastage. Because they are hydrophilic, it is logical to presume that they may
be effective in situations with minimal moisture contamination. Combining conditioning
and priming agents into a single treatment step results in reduced time and improved cost-
effectiveness for the clinician and indirectly for the patient.
These relatively new systems were used originally on dentin. Essentially, the
acidic part of the primer dissolves the smear layer and incorporates it into the mixture.
Acidic primer solutions also demineralizes the dentin and encapsulate the collagen fibers
and hydroxyapatite crystals. This simultaneous conditioning a